#------------------------------------------------------------------------------
#$Date: 2024-03-05 22:28:07 +0200 (Tue, 05 Mar 2024) $
#$Revision: 290317 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/31/24/2312408.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2312408
loop_
_publ_author_name
'Yoshino, Sho'
'Arima, Hidechika'
'Ishijima, Masanao'
'Kajihara, Koichi'
_publ_section_title
;
 Crystal structures of the alkali aluminoboracites
 A₄B₄Al₃O₁₂Cl (A
 = Li, Na).
;
_journal_coeditor_code           WM5704
_journal_issue                   'Pt 2'
_journal_name_full
'Acta crystallographica. Section E, Crystallographic communications'
_journal_page_first              169
_journal_page_last               173
_journal_paper_doi               10.1107/S2056989024000501
_journal_volume                  80
_journal_year                    2024
_chemical_formula_iupac          'Li4 B4 Al3 O12 Cl'
_chemical_formula_sum            'Al3 B4 Cl Li4 O12'
_chemical_formula_weight         379.39
_chemical_name_common            'Lithium aluminoboracite'
_chemical_name_systematic        'Lithium aluminoboracite'
_space_group_crystal_system      cubic
_space_group_IT_number           196
_space_group_name_Hall           'F 2 2 3'
_space_group_name_H-M_alt        'F 2 3'
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.98390(10)
_cell_length_b                   12.98390(10)
_cell_length_c                   12.98390(10)
_cell_measurement_reflns_used    2808
_cell_measurement_temperature    297(2)
_cell_measurement_theta_max      73.2152
_cell_measurement_theta_min      6.8200
_cell_volume                     2188.85(3)
_computing_cell_refinement
;
SAINT (Bruker, 2019)
;
_computing_data_collection
;
BIS (Bruker, 2021)
;
_computing_data_reduction
;
SAINT (Bruker, 2019)
;
_computing_molecular_graphics
;
VESTA (Momma & Izumi, 2011)
;
_computing_publication_material
;
publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXL (Sheldrick, 2015b) and ShelXle (Hübschle et al.,
2011)
;
_computing_structure_solution
;
SHELXTL (Sheldrick, 2015a)
;
_diffrn_ambient_temperature      297(2)
_diffrn_detector_area_resol_mean 7.3910
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8 goniometer'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0236
_diffrn_reflns_av_unetI/netI     0.0137
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            4728
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         73.208
_diffrn_reflns_theta_min         5.903
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    6.117
_exptl_absorpt_correction_T_max  0.75
_exptl_absorpt_correction_T_min  0.62
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(SADABS; Krause et al.,  2015)
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.303
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1472
_exptl_crystal_size_max          0.106
_exptl_crystal_size_mid          0.095
_exptl_crystal_size_min          0.059
_refine_diff_density_max         0.195
_refine_diff_density_min         -0.911
_refine_ls_abs_structure_details
;
Flack x determined using 132 quotients [(I+)-(I-)]/[(I+)+(I-)]
(Parsons et al.,  2013).
;
_refine_ls_abs_structure_Flack   -0.03(2)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.171
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     50
_refine_ls_number_reflns         389
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.169
_refine_ls_R_factor_all          0.0360
_refine_ls_R_factor_gt           0.0322
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0537P)²+1.5774P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0775
_refine_ls_wR_factor_ref         0.0814
_reflns_number_gt                317
_reflns_number_total             389
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            wm5704.cif
_cod_data_source_block           kjh0818yoshinoL14_0m_a_1
_cod_original_cell_volume        2188.85(5)
_cod_database_code               2312408
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Li Li1 0.020(4) 0.250000 0.250000 0.047(13) Uani d 0.5 . .
Li Li2 0.517(5) 0.750000 0.750000 0.050(15) Uani d 0.5 . .
Li Li3 0.363(3) 0.363(3) 0.363(3) 0.020(12) Uani d 0.205(14) . .
Li Li4 0.864(2) 0.864(2) 0.864(2) 0.035(12) Uani d 0.295(14) . .
B B1 0.1060(3) 0.1060(3) 0.1060(3) 0.0112(10) Uani d 1 . .
B B2 0.6057(3) 0.6057(3) 0.6057(3) 0.0119(10) Uani d 1 . .
Al Al1 0.24997(11) 0.000000 0.000000 0.0118(5) Uani d 1 . .
O O1 0.02797(13) 0.11005(14) 0.17683(14) 0.0170(5) Uani d 1 . .
O O2 0.02784(13) 0.17681(14) 0.61004(14) 0.0171(5) Uani d 1 . .
Cl Cl1 0.250000 0.250000 0.250000 0.0774(16) Uani d 1 . .
Cl Cl2 0.750000 0.750000 0.750000 0.0786(16) Uani d 1 . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.2130 0.2455 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0090 0.0039 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.3639 0.7018 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li 0.0008 0.0003 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Li2 Li1 O1 26_564 16 92.8(16) ?
Li2 Li1 O1 26_564 . 92.8(16) ?
O1 Li1 O1 16 . 174(3) ?
Li2 Li1 O2 26_564 14_554 73.1(14) ?
O1 Li1 O2 16 14_554 90.8(4) ?
O1 Li1 O2 . 14_554 90.8(4) ?
Li2 Li1 O2 26_564 3_556 73.1(14) ?
O1 Li1 O2 16 3_556 90.8(4) ?
O1 Li1 O2 . 3_556 90.8(4) ?
O2 Li1 O2 14_554 3_556 146(3) ?
Li2 Li1 Li3 26_564 27 126.0(15) ?
O1 Li1 Li3 16 27 74.3(8) ?
O1 Li1 Li3 . 27 102.3(12) ?
O2 Li1 Li3 14_554 27 55.4(12) ?
O2 Li1 Li3 3_556 27 155(2) ?
Li2 Li1 Li3 26_564 38 126.0(15) ?
O1 Li1 Li3 16 38 102.3(12) ?
O1 Li1 Li3 . 38 74.3(8) ?
O2 Li1 Li3 14_554 38 155(2) ?
O2 Li1 Li3 3_556 38 55.4(12) ?
Li3 Li1 Li3 27 38 108(3) ?
Li2 Li1 Li4 26_564 4_466 45.7(13) ?
O1 Li1 Li4 16 4_466 136(2) ?
O1 Li1 Li4 . 4_466 49.6(13) ?
O2 Li1 Li4 14_554 4_466 65.9(10) ?
O2 Li1 Li4 3_556 4_466 90.1(14) ?
Li3 Li1 Li4 27 4_466 114.3(10) ?
Li3 Li1 Li4 38 4_466 114.3(10) ?
Li2 Li1 Li4 26_564 13_444 45.7(13) ?
O1 Li1 Li4 16 13_444 49.6(13) ?
O1 Li1 Li4 . 13_444 136(2) ?
O2 Li1 Li4 14_554 13_444 90.1(14) ?
O2 Li1 Li4 3_556 13_444 65.9(10) ?
Li3 Li1 Li4 27 13_444 114.3(10) ?
Li3 Li1 Li4 38 13_444 114.3(10) ?
Li4 Li1 Li4 4_466 13_444 91(3) ?
Li2 Li1 Cl1 26_564 . 180.0 ?
O1 Li1 Cl1 16 . 87.2(16) ?
O1 Li1 Cl1 . . 87.2(16) ?
O2 Li1 Cl1 14_554 . 106.9(14) ?
O2 Li1 Cl1 3_556 . 106.9(14) ?
Li3 Li1 Cl1 27 . 54.0(15) ?
Li3 Li1 Cl1 38 . 54.0(15) ?
Li4 Li1 Cl1 4_466 . 134.3(13) ?
Li4 Li1 Cl1 13_444 . 134.3(13) ?
Li2 Li1 Al1 26_564 9 85.4(10) ?
O1 Li1 Al1 16 9 152.41(19) ?
O1 Li1 Al1 . 9 28.56(17) ?
O2 Li1 Al1 14_554 9 114.7(7) ?
O2 Li1 Al1 3_556 9 62.3(2) ?
Li3 Li1 Al1 27 9 128.1(12) ?
Li3 Li1 Al1 38 9 58.5(7) ?
Li4 Li1 Al1 4_466 9 55.9(7) ?
Li4 Li1 Al1 13_444 9 116.6(14) ?
Cl1 Li1 Al1 . 9 94.6(10) ?
Li2 Li1 Al1 26_564 5 85.4(10) ?
O1 Li1 Al1 16 5 117.73(11) ?
O1 Li1 Al1 . 5 62.78(10) ?
O2 Li1 Al1 14_554 5 29.72(10) ?
O2 Li1 Al1 3_556 5 145.3(15) ?
Li3 Li1 Al1 27 5 58.5(7) ?
Li3 Li1 Al1 38 5 128.1(12) ?
Li4 Li1 Al1 4_466 5 55.9(7) ?
Li4 Li1 Al1 13_444 5 116.6(14) ?
Cl1 Li1 Al1 . 5 94.6(10) ?
Al1 Li1 Al1 9 5 89.62(17) ?
O2 Li2 O2 28_566 37 172(3) ?
O2 Li2 O1 28_566 39_556 91.1(4) ?
O2 Li2 O1 37 39_556 91.1(4) ?
O2 Li2 O1 28_566 26_565 91.1(4) ?
O2 Li2 O1 37 26_565 91.1(4) ?
O1 Li2 O1 39_556 26_565 148(3) ?
O2 Li2 Li4 28_566 27_656 101.4(13) ?
O2 Li2 Li4 37 27_656 73.7(9) ?
O1 Li2 Li4 39_556 27_656 154(2) ?
O1 Li2 Li4 26_565 27_656 55.1(12) ?
O2 Li2 Li4 28_566 38_665 73.7(9) ?
O2 Li2 Li4 37 38_665 101.4(13) ?
O1 Li2 Li4 39_556 38_665 55.1(12) ?
O1 Li2 Li4 26_565 38_665 154(2) ?
Li4 Li2 Li4 27_656 38_665 107(3) ?
O2 Li2 Li3 28_566 4_566 137(2) ?
O2 Li2 Li3 37 4_566 50.2(14) ?
O1 Li2 Li3 39_556 4_566 66.6(10) ?
O1 Li2 Li3 26_565 4_566 91.1(15) ?
Li4 Li2 Li3 27_656 4_566 114.4(10) ?
Li4 Li2 Li3 38_665 4_566 114.4(10) ?
O2 Li2 Li3 28_566 13 50.2(13) ?
O2 Li2 Li3 37 13 137(2) ?
O1 Li2 Li3 39_556 13 91.1(15) ?
O1 Li2 Li3 26_565 13 66.6(10) ?
Li4 Li2 Li3 27_656 13 114.4(10) ?
Li4 Li2 Li3 38_665 13 114.4(10) ?
Li3 Li2 Li3 4_566 13 92(3) ?
O2 Li2 Cl2 28_566 . 86.0(17) ?
O2 Li2 Cl2 37 . 86.0(17) ?
O1 Li2 Cl2 39_556 . 105.9(15) ?
O1 Li2 Cl2 26_565 . 105.9(15) ?
Li4 Li2 Cl2 27_656 . 53.3(15) ?
Li4 Li2 Cl2 38_665 . 53.3(15) ?
Li3 Li2 Cl2 4_566 . 133.8(13) ?
Li3 Li2 Cl2 13 . 133.8(13) ?
O2 Li2 Al1 28_566 46_556 117.76(6) ?
O2 Li2 Al1 37 46_556 62.84(9) ?
O1 Li2 Al1 39_556 46_556 29.66(11) ?
O1 Li2 Al1 26_565 46_556 146.3(15) ?
Li4 Li2 Al1 27_656 46_556 127.3(13) ?
Li4 Li2 Al1 38_665 46_556 58.3(7) ?
Li3 Li2 Al1 4_566 46_556 56.2(7) ?
Li3 Li2 Al1 13 46_556 117.5(15) ?
Cl2 Li2 Al1 . 46_556 93.9(10) ?
O2 Li2 Al1 28_566 30_565 152.45(6) ?
O2 Li2 Al1 37 30_565 28.68(17) ?
O1 Li2 Al1 39_556 30_565 115.2(7) ?
O1 Li2 Al1 26_565 30_565 62.41(19) ?
Li4 Li2 Al1 27_656 30_565 58.3(7) ?
Li4 Li2 Al1 38_665 30_565 127.3(13) ?
Li3 Li2 Al1 4_566 30_565 56.2(7) ?
Li3 Li2 Al1 13 30_565 117.5(15) ?
Cl2 Li2 Al1 . 30_565 93.9(10) ?
Al1 Li2 Al1 46_556 30_565 89.75(15) ?
O2 Li2 Al1 28_566 41_556 28.68(17) ?
O2 Li2 Al1 37 41_556 152.45(6) ?
O1 Li2 Al1 39_556 41_556 62.41(19) ?
O1 Li2 Al1 26_565 41_556 115.2(7) ?
Li4 Li2 Al1 27_656 41_556 127.3(13) ?
Li4 Li2 Al1 38_665 41_556 58.3(7) ?
Li3 Li2 Al1 4_566 41_556 117.5(15) ?
Li3 Li2 Al1 13 41_556 56.2(7) ?
Cl2 Li2 Al1 . 41_556 93.9(10) ?
Al1 Li2 Al1 46_556 41_556 89.73(15) ?
Al1 Li2 Al1 30_565 41_556 172(2) ?
O2 Li3 O2 20_655 36_565 96.4(16) ?
O2 Li3 O2 20_655 40_556 96.4(16) ?
O2 Li3 O2 36_565 40_556 96.4(16) ?
O2 Li3 Cl1 20_655 . 120.6(12) ?
O2 Li3 Cl1 36_565 . 120.6(12) ?
O2 Li3 Cl1 40_556 . 120.6(12) ?
O2 Li3 Li1 20_655 38 108.9(5) ?
O2 Li3 Li1 36_565 38 140.8(8) ?
O2 Li3 Li1 40_556 38 52.5(10) ?
Cl1 Li3 Li1 . 38 71.3(15) ?
O2 Li3 Li1 20_655 18 52.4(10) ?
O2 Li3 Li1 36_565 18 108.9(5) ?
O2 Li3 Li1 40_556 18 140.8(8) ?
Cl1 Li3 Li1 . 18 71.3(15) ?
Li1 Li3 Li1 38 18 110.2(15) ?
O2 Li3 Li1 20_655 34 140.8(8) ?
O2 Li3 Li1 36_565 34 52.4(10) ?
O2 Li3 Li1 40_556 34 108.9(5) ?
Cl1 Li3 Li1 . 34 71.3(15) ?
Li1 Li3 Li1 38 34 110.2(15) ?
Li1 Li3 Li1 18 34 110.2(15) ?
O2 Li3 O1 20_655 34 157(2) ?
O2 Li3 O1 36_565 34 71.5(2) ?
O2 Li3 O1 40_556 34 66.68(17) ?
Cl1 Li3 O1 . 34 82.2(11) ?
Li1 Li3 O1 38 34 74.0(4) ?
Li1 Li3 O1 18 34 149(2) ?
Li1 Li3 O1 34 34 44.4(3) ?
O2 Li3 O1 20_655 18 71.5(2) ?
O2 Li3 O1 36_565 18 66.68(17) ?
O2 Li3 O1 40_556 18 157(2) ?
Cl1 Li3 O1 . 18 82.2(11) ?
Li1 Li3 O1 38 18 149(2) ?
Li1 Li3 O1 18 18 44.4(3) ?
Li1 Li3 O1 34 18 73.9(4) ?
O1 Li3 O1 34 18 118.2(5) ?
O2 Li3 O1 20_655 38 66.68(17) ?
O2 Li3 O1 36_565 38 157(2) ?
O2 Li3 O1 40_556 38 71.5(2) ?
Cl1 Li3 O1 . 38 82.2(11) ?
Li1 Li3 O1 38 38 44.4(3) ?
Li1 Li3 O1 18 38 73.9(4) ?
Li1 Li3 O1 34 38 149(2) ?
O1 Li3 O1 34 38 118.2(5) ?
O1 Li3 O1 18 38 118.2(5) ?
O2 Li3 Li2 20_655 29_454 45.2(8) ?
O2 Li3 Li2 36_565 29_454 105.2(6) ?
O2 Li3 Li2 40_556 29_454 137.0(11) ?
Cl1 Li3 Li2 . 29_454 79.1(13) ?
Li1 Li3 Li2 38 29_454 113.8(9) ?
Li1 Li3 Li2 18 29_454 7.8(17) ?
Li1 Li3 Li2 34 29_454 113.8(9) ?
O1 Li3 Li2 34 29_454 155.6(18) ?
O1 Li3 Li2 18 29_454 43.86(15) ?
O1 Li3 Li2 38 29_454 74.5(3) ?
O2 Li3 Li2 20_655 13_544 105.2(6) ?
O2 Li3 Li2 36_565 13_544 137.0(11) ?
O2 Li3 Li2 40_556 13_544 45.2(8) ?
Cl1 Li3 Li2 . 13_544 79.1(13) ?
Li1 Li3 Li2 38 13_544 7.8(17) ?
Li1 Li3 Li2 18 13_544 113.8(9) ?
Li1 Li3 Li2 34 13_544 113.8(9) ?
O1 Li3 Li2 34 13_544 74.5(3) ?
O1 Li3 Li2 18 13_544 155.6(18) ?
O1 Li3 Li2 38 13_544 43.86(15) ?
Li2 Li3 Li2 29_454 13_544 116.5(8) ?
O1 Li4 O1 8_666 4_666 96.6(15) ?
O1 Li4 O1 8_666 12_666 96.6(15) ?
O1 Li4 O1 4_666 12_666 96.6(15) ?
O1 Li4 Cl2 8_666 . 120.5(12) ?
O1 Li4 Cl2 4_666 . 120.5(12) ?
O1 Li4 Cl2 12_666 . 120.5(12) ?
O1 Li4 Li2 8_666 38_665 140.6(8) ?
O1 Li4 Li2 4_666 38_665 51.7(10) ?
O1 Li4 Li2 12_666 38_665 108.6(5) ?
Cl2 Li4 Li2 . 38_665 71.9(15) ?
O1 Li4 Li2 8_666 34_656 108.6(5) ?
O1 Li4 Li2 4_666 34_656 140.6(8) ?
O1 Li4 Li2 12_666 34_656 51.7(10) ?
Cl2 Li4 Li2 . 34_656 71.9(15) ?
Li2 Li4 Li2 38_665 34_656 110.8(14) ?
O1 Li4 Li2 8_666 18_566 51.7(10) ?
O1 Li4 Li2 4_666 18_566 108.6(5) ?
O1 Li4 Li2 12_666 18_566 140.6(8) ?
Cl2 Li4 Li2 . 18_566 71.9(15) ?
Li2 Li4 Li2 38_665 18_566 110.8(14) ?
Li2 Li4 Li2 34_656 18_566 110.9(14) ?
O1 Li4 O2 8_666 15_656 157(2) ?
O1 Li4 O2 4_666 15_656 71.5(2) ?
O1 Li4 O2 12_666 15_656 66.70(16) ?
Cl2 Li4 O2 . 15_656 82.1(11) ?
Li2 Li4 O2 38_665 15_656 44.3(2) ?
Li2 Li4 O2 34_656 15_656 74.0(4) ?
Li2 Li4 O2 18_566 15_656 150(2) ?
O1 Li4 O2 8_666 47_566 66.70(16) ?
O1 Li4 O2 4_666 47_566 157(2) ?
O1 Li4 O2 12_666 47_566 71.5(2) ?
Cl2 Li4 O2 . 47_566 82.1(11) ?
Li2 Li4 O2 38_665 47_566 150(2) ?
Li2 Li4 O2 34_656 47_566 44.3(2) ?
Li2 Li4 O2 18_566 47_566 74.0(4) ?
O2 Li4 O2 15_656 47_566 118.2(5) ?
O1 Li4 O2 8_666 31_665 71.5(2) ?
O1 Li4 O2 4_666 31_665 66.70(16) ?
O1 Li4 O2 12_666 31_665 157(2) ?
Cl2 Li4 O2 . 31_665 82.1(11) ?
Li2 Li4 O2 38_665 31_665 74.0(4) ?
Li2 Li4 O2 34_656 31_665 150(2) ?
Li2 Li4 O2 18_566 31_665 44.3(2) ?
O2 Li4 O2 15_656 31_665 118.2(5) ?
O2 Li4 O2 47_566 31_665 118.2(5) ?
O1 Li4 Al1 8_666 10_666 68.7(7) ?
O1 Li4 Al1 4_666 10_666 37.0(3) ?
O1 Li4 Al1 12_666 10_666 122(2) ?
Cl2 Li4 Al1 . 10_666 114.3(9) ?
Li2 Li4 Al1 38_665 10_666 72.2(6) ?
Li2 Li4 Al1 34_656 10_666 174(2) ?
Li2 Li4 Al1 18_566 10_666 72.2(6) ?
O2 Li4 Al1 15_656 10_666 106.3(4) ?
O2 Li4 Al1 47_566 10_666 134.6(7) ?
O2 Li4 Al1 31_665 10_666 35.59(12) ?
O1 Li4 Al1 8_666 2_666 37.0(3) ?
O1 Li4 Al1 4_666 2_666 122(2) ?
O1 Li4 Al1 12_666 2_666 68.7(7) ?
Cl2 Li4 Al1 . 2_666 114.3(9) ?
Li2 Li4 Al1 38_665 2_666 174(2) ?
Li2 Li4 Al1 34_656 2_666 72.2(6) ?
Li2 Li4 Al1 18_566 2_666 72.2(6) ?
O2 Li4 Al1 15_656 2_666 134.6(7) ?
O2 Li4 Al1 47_566 2_666 35.59(12) ?
O2 Li4 Al1 31_665 2_666 106.3(4) ?
Al1 Li4 Al1 10_666 2_666 104.3(11) ?
O1 B1 O1 . 9 119.972(15) ?
O1 B1 O1 . 5 119.972(15) ?
O1 B1 O1 9 5 119.972(15) ?
O2 B2 O2 33 37 119.982(12) ?
O2 B2 O2 33 17 119.982(13) ?
O2 B2 O2 37 17 119.982(12) ?
O1 Al1 O2 6 46_545 107.12(9) ?
O1 Al1 O1 6 5 114.42(15) ?
O2 Al1 O1 46_545 5 107.03(8) ?
O1 Al1 O2 6 48 107.03(8) ?
O2 Al1 O2 46_545 48 114.35(15) ?
O1 Al1 O2 5 48 107.12(9) ?
O1 Al1 Li4 6 3_646 95.5(7) ?
O2 Al1 Li4 46_545 3_646 153.8(2) ?
O1 Al1 Li4 5 3_646 49.8(3) ?
O2 Al1 Li4 48 3_646 69.7(8) ?
O1 Al1 Li4 6 2_664 49.8(3) ?
O2 Al1 Li4 46_545 2_664 69.7(8) ?
O1 Al1 Li4 5 2_664 95.5(7) ?
O2 Al1 Li4 48 2_664 153.8(2) ?
Li4 Al1 Li4 3_646 2_664 119.1(19) ?
O1 Al1 Li3 6 16 153.8(2) ?
O2 Al1 Li3 46_545 16 49.8(3) ?
O1 Al1 Li3 5 16 69.5(9) ?
O2 Al1 Li3 48 16 95.6(7) ?
Li4 Al1 Li3 3_646 16 104.9(7) ?
Li4 Al1 Li3 2_664 16 104.9(7) ?
O1 Al1 Li3 6 13_544 69.5(9) ?
O2 Al1 Li3 46_545 13_544 95.6(7) ?
O1 Al1 Li3 5 13_544 153.8(2) ?
O2 Al1 Li3 48 13_544 49.8(3) ?
Li4 Al1 Li3 3_646 13_544 104.9(7) ?
Li4 Al1 Li3 2_664 13_544 104.9(7) ?
Li3 Al1 Li3 16 13_544 119(2) ?
O1 Al1 Li2 6 41_444 37.0(5) ?
O2 Al1 Li2 46_545 41_444 74.9(9) ?
O1 Al1 Li2 5 41_444 143.0(5) ?
O2 Al1 Li2 48 41_444 105.1(9) ?
Li4 Al1 Li2 3_646 41_444 130.5(9) ?
Li4 Al1 Li2 2_664 41_444 49.5(9) ?
Li3 Al1 Li2 16 41_444 124.6(9) ?
Li3 Al1 Li2 13_544 41_444 55.4(9) ?
O1 Al1 Li2 6 22_645 98.7(9) ?
O2 Al1 Li2 46_545 22_645 34.2(3) ?
O1 Al1 Li2 5 22_645 81.3(9) ?
O2 Al1 Li2 48 22_645 145.8(3) ?
Li4 Al1 Li2 3_646 22_645 130.5(9) ?
Li4 Al1 Li2 2_664 22_645 49.5(9) ?
Li3 Al1 Li2 16 22_645 55.4(9) ?
Li3 Al1 Li2 13_544 22_645 124.6(9) ?
Li2 Al1 Li2 41_444 22_645 82(2) ?
O1 Al1 Li2 6 33_444 81.3(9) ?
O2 Al1 Li2 46_545 33_444 145.8(3) ?
O1 Al1 Li2 5 33_444 98.7(9) ?
O2 Al1 Li2 48 33_444 34.2(3) ?
Li4 Al1 Li2 3_646 33_444 49.5(9) ?
Li4 Al1 Li2 2_664 33_444 130.5(9) ?
Li3 Al1 Li2 16 33_444 124.6(9) ?
Li3 Al1 Li2 13_544 33_444 55.4(9) ?
Li2 Al1 Li2 41_444 33_444 98(2) ?
Li2 Al1 Li2 22_645 33_444 179.99(5) ?
O1 Al1 Li2 6 42_456 143.0(5) ?
O2 Al1 Li2 46_545 42_456 105.1(9) ?
O1 Al1 Li2 5 42_456 37.0(5) ?
O2 Al1 Li2 48 42_456 74.9(9) ?
Li4 Al1 Li2 3_646 42_456 49.5(9) ?
Li4 Al1 Li2 2_664 42_456 130.5(9) ?
Li3 Al1 Li2 16 42_456 55.4(9) ?
Li3 Al1 Li2 13_544 42_456 124.6(9) ?
Li2 Al1 Li2 41_444 42_456 180.0(17) ?
Li2 Al1 Li2 22_645 42_456 98(2) ?
Li2 Al1 Li2 33_444 42_456 82(2) ?
B1 O1 Al1 . 9 119.05(13) ?
B1 O1 Li1 . . 112.4(12) ?
Al1 O1 Li1 9 . 117.4(4) ?
B1 O1 Li2 . 26_564 122.3(12) ?
Al1 O1 Li2 9 26_564 113.4(6) ?
Li1 O1 Li2 . 26_564 13(3) ?
B1 O1 Li4 . 4_466 123.9(9) ?
Al1 O1 Li4 9 4_466 93.12(8) ?
Li1 O1 Li4 . 4_466 85.7(19) ?
Li2 O1 Li4 26_564 4_466 73.2(19) ?
B1 O1 Li3 . 38 102.2(9) ?
Al1 O1 Li3 9 38 74.9(10) ?
Li1 O1 Li3 . 38 61.3(10) ?
Li2 O1 Li3 26_564 38 69.5(10) ?
Li4 O1 Li3 4_466 38 131.5(12) ?
B1 O1 Li3 . . 75.8(3) ?
Al1 O1 Li3 9 . 112.35(10) ?
Li1 O1 Li3 . . 50.3(16) ?
Li2 O1 Li3 26_564 . 63.2(15) ?
Li4 O1 Li3 4_466 . 135.3(9) ?
Li3 O1 Li3 38 . 38.8(10) ?
B2 O2 Al1 37_445 18 118.94(13) ?
B2 O2 Li2 37_445 37_445 113.5(13) ?
Al1 O2 Li2 18 37_445 117.1(5) ?
B2 O2 Li1 37_445 14 123.2(11) ?
Al1 O2 Li1 18 14 113.0(5) ?
Li2 O2 Li1 37_445 14 13(3) ?
B2 O2 Li3 37_445 40_456 123.8(10) ?
Al1 O2 Li3 18 40_456 93.19(8) ?
Li2 O2 Li3 37_445 40_456 85(2) ?
Li1 O2 Li3 14 40_456 72.1(18) ?
B2 O2 Li4 37_445 15_646 102.4(9) ?
Al1 O2 Li4 18 15_646 74.7(10) ?
Li2 O2 Li4 37_445 15_646 62.0(11) ?
Li1 O2 Li4 14 15_646 70.2(10) ?
Li3 O2 Li4 40_456 15_646 131.4(12) ?
B2 O2 Li4 37_445 . 82.6(3) ?
Al1 O2 Li4 18 . 90.33(9) ?
Li2 O2 Li4 37_445 . 64.2(14) ?
Li1 O2 Li4 14 . 75.6(13) ?
Li3 O2 Li4 40_456 . 146.2(12) ?
Li4 O2 Li4 15_646 . 21.0(10) ?
Li3 Cl1 Li3 . 16 109.468(7) ?
Li3 Cl1 Li3 . 27 109.473(3) ?
Li3 Cl1 Li3 16 27 109.4730(10) ?
Li3 Cl1 Li3 . 38 109.4730(10) ?
Li3 Cl1 Li3 16 38 109.5 ?
Li3 Cl1 Li3 27 38 109.468(2) ?
Li3 Cl1 Li1 . . 125.2660(10) ?
Li3 Cl1 Li1 16 . 125.266(4) ?
Li3 Cl1 Li1 27 . 54.7340(10) ?
Li3 Cl1 Li1 38 . 54.734(2) ?
Li3 Cl1 Li1 . 18 54.736(2) ?
Li3 Cl1 Li1 16 18 125.264(3) ?
Li3 Cl1 Li1 27 18 54.736(2) ?
Li3 Cl1 Li1 38 18 125.264(2) ?
Li1 Cl1 Li1 . 18 90.000(3) ?
Li3 Cl1 Li1 . 9 125.264(5) ?
Li3 Cl1 Li1 16 9 54.7360(10) ?
Li3 Cl1 Li1 27 9 54.736(2) ?
Li3 Cl1 Li1 38 9 125.264(4) ?
Li1 Cl1 Li1 . 9 90.000(3) ?
Li1 Cl1 Li1 18 9 90.0 ?
Li3 Cl1 Li1 . 34 54.736(2) ?
Li3 Cl1 Li1 16 34 125.2640(10) ?
Li3 Cl1 Li1 27 34 125.264(2) ?
Li3 Cl1 Li1 38 34 54.736(2) ?
Li1 Cl1 Li1 . 34 90.000(3) ?
Li1 Cl1 Li1 18 34 90.0 ?
Li1 Cl1 Li1 9 34 180.0 ?
Li3 Cl1 Li1 . 5 125.2640(10) ?
Li3 Cl1 Li1 16 5 54.7360(10) ?
Li3 Cl1 Li1 27 5 125.264(4) ?
Li3 Cl1 Li1 38 5 54.7360(10) ?
Li1 Cl1 Li1 . 5 90.000(4) ?
Li1 Cl1 Li1 18 5 180.0 ?
Li1 Cl1 Li1 9 5 90.000(2) ?
Li1 Cl1 Li1 34 5 90.0 ?
Li3 Cl1 Li1 . 38 54.734(2) ?
Li3 Cl1 Li1 16 38 54.734(3) ?
Li3 Cl1 Li1 27 38 125.266(2) ?
Li3 Cl1 Li1 38 38 125.2660(10) ?
Li1 Cl1 Li1 . 38 180.0 ?
Li1 Cl1 Li1 18 38 90.000(5) ?
Li1 Cl1 Li1 9 38 90.0 ?
Li1 Cl1 Li1 34 38 90.000(4) ?
Li1 Cl1 Li1 5 38 90.0000(10) ?
Li4 Cl2 Li4 . 16_566 109.474(11) ?
Li4 Cl2 Li4 . 38_665 109.470(2) ?
Li4 Cl2 Li4 16_566 38_665 109.470(3) ?
Li4 Cl2 Li4 . 27_656 109.470(6) ?
Li4 Cl2 Li4 16_566 27_656 109.5 ?
Li4 Cl2 Li4 38_665 27_656 109.474(7) ?
Li4 Cl2 Li2 . . 125.263(4) ?
Li4 Cl2 Li2 16_566 . 125.263(12) ?
Li4 Cl2 Li2 38_665 . 54.737(7) ?
Li4 Cl2 Li2 27_656 . 54.737(6) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Li1 Li2 26_564 0.48(10) ?
Li1 O1 16 2.053(3) ?
Li1 O1 . 2.053(3) ?
Li1 O2 14_554 2.143(16) ?
Li1 O2 3_556 2.143(16) ?
Li1 Li3 27 2.57(4) ?
Li1 Li3 38 2.57(4) ?
Li1 Li4 4_466 2.91(4) ?
Li1 Li4 13_444 2.91(4) ?
Li1 Cl1 . 2.98(6) ?
Li1 Al1 9 3.256(5) ?
Li1 Al1 5 3.256(5) ?
Li2 O2 28_566 2.056(4) ?
Li2 O2 37 2.056(4) ?
Li2 O1 39_556 2.132(16) ?
Li2 O1 26_565 2.132(16) ?
Li2 Li4 27_656 2.60(4) ?
Li2 Li4 38_665 2.60(4) ?
Li2 Li3 4_566 2.88(4) ?
Li2 Li3 13 2.88(4) ?
Li2 Cl2 . 3.03(6) ?
Li2 Al1 46_556 3.253(4) ?
Li2 Al1 30_565 3.253(4) ?
Li2 Al1 41_556 3.253(4) ?
Li3 O2 20_655 2.23(3) ?
Li3 O2 36_565 2.23(3) ?
Li3 O2 40_556 2.23(3) ?
Li3 Cl1 . 2.55(6) ?
Li3 O1 34 2.824(8) ?
Li3 O1 18 2.824(8) ?
Li3 O1 38 2.824(8) ?
Li4 O1 8_666 2.23(3) ?
Li4 O1 4_666 2.23(3) ?
Li4 O1 12_666 2.23(3) ?
Li4 Cl2 . 2.55(5) ?
Li4 O2 15_656 2.826(8) ?
Li4 O2 47_566 2.826(8) ?
Li4 O2 31_665 2.826(8) ?
Li4 Al1 10_666 2.91(2) ?
Li4 Al1 2_666 2.91(2) ?
B1 O1 . 1.3693(17) ?
B1 O1 9 1.3693(17) ?
B1 O1 5 1.3693(17) ?
B2 O2 33 1.3702(17) ?
B2 O2 37 1.3702(17) ?
B2 O2 17 1.3702(17) ?
Al1 O1 6 1.754(2) ?
Al1 O2 46_545 1.754(2) ?
Al1 O1 5 1.754(2) ?
Al1 O2 48 1.754(2) ?
